3Estonian Nanotechnology Competence Centre, Riia 142, 51014
Silver nanowires for transparent conductive electrodes:
In situ mechanical characterization
Boris Polyakov1,3, Sergei Vlassov2,3, Leonid Dorogin2,3, Mikk Antsov2,3, Ilmar Kink2,3, Runno Lohmus2,3
of Solid State Physics, University of Latvia, Kengaraga 8, LV-1063, Riga, Latvia
of Physics, University of Tartu, Riia 142, 51014, Tartu, Estonia
3Estonian Nanotechnology Competence Centre, Riia 142, 51014, Tartu, Estonia
Recently, flexible and stretchable electronics based on nanomaterials have received much recent
attention as an alternative of transparent conducive oxide coatings for wide range of applications,
including thin film solar cells, displays, organic light-emitting diodes, etc. Two dimensional networks of
metal nanowires (NWs) can form a high-performance transparent conducting film that could be coated
by different methods from a liquid solvent, and significantly reduce production costs. For example,
solution-coated films of silver NWs have a transmittance and sheet resistance close to ITO .
There are several works, where mechanical properties of silver NWs were investigated, such as
micro hardness, Young modulus, tensile strength in axial stretching and three point bending tests [2, 3,
4]. However, to the best of our knowledge, pure bending tests of Ag NWs were not reported in literature
In this work, we describe bending tests inside a SEM chamber, which enables the measurement
of the Young modulus and yield strength of NWs, and monitor elastic and plastic deformation in real
time. Silver NW half-suspended on edge of micro machined silicon grating was pushed by AFM tip
glued to a quartz tuning fork (QTF) mounted on a nanomanipulator (fig.1). The NW-tip force interaction
detected by a QTF force sensor and corresponding to the visualized by SEM NW’s bending was used to
calculate Young modulus and yield strength, similar experimental setup used in .
Bending tests were performed on 20 NWs with diameters ranging from 76 nm to 211 nm.
Typically two regions were clearly distinguished on bending curves as shown on fig. 2. In initial region
(a-b) NW bends elastically and the force grows linearly with a bending angle of NW. It was also
confirmed separately on several NWs that in the linear region removal of external force will cause NW to
return in initial no deformed state (elastic deformation regime). At certain point deformation turns to
plastic. The onset of elastic-to-plastic transition can be detected precisely from the change of slope of
the force curve (point b). From this point bending continues with a nearly constant force (region b-c)
corresponding to plastic yield of the wire. Some NWs demonstrated slightly different behavior during
bending test due to crack formation (fig. 3). Formation of crack inside NW manifests itself as clear steps
on force curve. In some cases crack stabilizes and stops propagating, in other cases NWs break
We found Young modulus of Ag NWs was 90±29 GPa. Additionally, fatigue tests with several
millions of cycles were performed and it was demonstrated that Ag NWs have high fatigue resistance
and can be bent elastically multiple times to significant curvatures without failure.
 L. Hu , H. Wu , Y. Cui, Metal nanogrids, nanowires, and nanofibers for transparent electrodes. MRS
Bulletin 36 (2011) 760-765
 X. Li, H. Gao, C. Murphy, K. Caswell,Nanoindentation of Silver Nanowires. Nanolett. 3 (2003) 14951498
 Y. Zhu, Q. Qin, F. Xu, F. Fan, Y. Ding, T. Zhang, B.Wiley, Z. Wang. Size effects on elasticity,
yielding, and fracture of silver nanowires: In situ experiments. Phys. Rev. B 85 (2012) 045443
 B. Wu, A. Heidelberg, J. Boland, J. Sader, X. Sun, Y. Li, Microstructure-Hardened Silver
Nanowires. Nanolett. 6 (2006) 468-472
 B.Polyakov, L.Dorogin, S.Vlassov, M.Antsov, P.Kulis, I.Kink, R. Lohmus. In situ measurements of
ultimate bending strength of CuO and ZnO nanowires. Europ. Phys. J. B. 85 (2012) 366
Figure 1. Schematics of experiment setup inside SEM. AFM tip glued on QTF pushes a silver NW on
Figure 2. Bending test of Ag NW. Set of four SEM images and corresponding force registered
simultaneously by force sensor. Tip approaches a NW (a). Maximal elastic deformation of NW (b).
Plastic deformation regime (c). Retraction of the tip (d). Force curve of NW deformation (e).
Figure 3. SEM images of plastically deformed Ag NWs. Bend without cracking (a). Cracked during